#------------------------------------------------------------------------------
#$Date: 2016-02-16 22:30:59 +0200 (Tue, 16 Feb 2016) $
#$Revision: 176467 $
#$URL: svn://www.crystallography.net/cod/cif/4/32/88/4328818.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4328818
loop_
_publ_author_name
'Karah E. Knope'
'Monica Vasiliu'
'David A. Dixon'
'L. Soderholm'
_publ_contact_author_address
;
Chemical Sciences and Engineering Division
Argonne National Laboratory
9700 South Cass Avenue
Argonne, IL 60439
;
_publ_contact_author_email       ls@anl.gov
_publ_contact_author_name        'L. Soderholm'
_publ_contact_author_phone       630-252-4364
_publ_section_title
;
 Thorium(IV)-Selenate Clusters Containing an Octanuclear Th(IV)
 Hydroxide/Oxide Core
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              4239
_journal_page_last               4249
_journal_paper_doi               10.1021/ic202706s
_journal_volume                  51
_journal_year                    2012
_chemical_formula_moiety         'H38 O59 Se8 Th8, 7.5(H2O)'
_chemical_formula_sum            'H52 O66.5 Se8 Th8'
_chemical_formula_weight         3604.42
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           2
_symmetry_cell_setting           triclinic
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_atom_sites_solution_hydrogens   notdet
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                97.3200(10)
_cell_angle_beta                 94.9890(10)
_cell_angle_gamma                109.7880(10)
_cell_formula_units_Z            2
_cell_length_a                   9.2227(6)
_cell_length_b                   13.1858(9)
_cell_length_c                   25.1444(17)
_cell_measurement_reflns_used    9929
_cell_measurement_temperature    100(2)
_cell_measurement_theta_max      33.14
_cell_measurement_theta_min      4.44
_cell_volume                     2825.9(3)
_computing_cell_refinement       'Bruker Apex2'
_computing_data_collection       'Bruker Apex2'
_computing_data_reduction        'Bruker SAINT'
_computing_molecular_graphics    CrystalMaker
_computing_publication_material  'WinGX v1.80.05'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 2008)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 2008)'
_diffrn_ambient_temperature      100(2)
_diffrn_measured_fraction_theta_full 0.995
_diffrn_measured_fraction_theta_max 0.962
_diffrn_measurement_device_type  'Bruker ApexII CCD'
_diffrn_measurement_method       'omega scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0582
_diffrn_reflns_av_sigmaI/netI    0.0845
_diffrn_reflns_limit_h_max       14
_diffrn_reflns_limit_h_min       -14
_diffrn_reflns_limit_k_max       20
_diffrn_reflns_limit_k_min       -20
_diffrn_reflns_limit_l_max       38
_diffrn_reflns_limit_l_min       -38
_diffrn_reflns_number            49686
_diffrn_reflns_theta_full        25.25
_diffrn_reflns_theta_max         33.22
_diffrn_reflns_theta_min         3.99
_exptl_absorpt_coefficient_mu    26.262
_exptl_absorpt_correction_T_max  0.7456
_exptl_absorpt_correction_T_min  0.5048
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   SADABS
_exptl_crystal_colour            colorless
_exptl_crystal_density_diffrn    4.236
_exptl_crystal_description       block
_exptl_crystal_F_000             3152
_exptl_crystal_size_max          0.08
_exptl_crystal_size_mid          0.07
_exptl_crystal_size_min          0.04
_refine_diff_density_max         2.752
_refine_diff_density_min         -2.811
_refine_diff_density_rms         0.506
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   0.978
_refine_ls_hydrogen_treatment    noref
_refine_ls_matrix_type           full
_refine_ls_number_parameters     758
_refine_ls_number_reflns         20858
_refine_ls_number_restraints     867
_refine_ls_restrained_S_all      0.961
_refine_ls_R_factor_all          0.0701
_refine_ls_R_factor_gt           0.0420
_refine_ls_shift/su_max          0.003
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0273P)²+0.0000P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0778
_refine_ls_wR_factor_ref         0.0866
_reflns_number_gt                14995
_reflns_number_total             20858
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic202706s_si_002_2.cif
_cod_data_source_block           H52O66.5Se8Th8
_cod_original_formula_sum        'H52 O66.50 Se8 Th8'
_cod_database_code               4328818
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, -z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Th1 Th 0.93547(3) 0.43144(2) 0.824444(12) 0.00552(6) Uani 1 1 d U . .
Th2 Th 0.89477(3) 0.41158(2) 0.655530(12) 0.00519(6) Uani 1 1 d U . .
Th3 Th 1.12675(3) 0.77401(2) 0.842024(12) 0.00558(6) Uani 1 1 d U . .
Th4 Th 1.06843(3) 0.75379(2) 0.674111(12) 0.00579(6) Uani 1 1 d U . .
Th5 Th 0.54159(3) 0.28852(2) 0.730099(12) 0.00573(6) Uani 1 1 d U . .
Th6 Th 1.26620(3) 0.57577(2) 0.598455(12) 0.00558(6) Uani 1 1 d U . .
Th7 Th 0.86238(3) 0.90194(2) 0.766987(12) 0.00632(6) Uani 1 1 d U . .
Th8 Th 1.34947(3) 0.59991(2) 0.897990(12) 0.00614(6) Uani 1 1 d U . .
O1 O 1.0685(6) 0.5825(4) 0.6479(2) 0.0059(9) Uani 1 1 d U . .
O2 O 0.8052(6) 0.3844(4) 0.7371(2) 0.0062(9) Uani 1 1 d U . .
O3 O 1.1269(6) 0.6017(4) 0.8502(2) 0.0058(9) Uani 1 1 d U . .
O4 O 1.0217(7) 0.8001(4) 0.7607(2) 0.0069(9) Uani 1 1 d U . .
O5 O 0.9491(7) 0.8719(5) 0.8525(2) 0.0110(11) Uani 1 1 d U . .
O6 O 0.8862(7) 0.8466(5) 0.6773(2) 0.0121(11) Uani 1 1 d U . .
O7 O 1.2950(7) 0.7578(5) 0.6333(2) 0.0096(10) Uani 1 1 d U . .
O8 O 1.1088(7) 0.3999(5) 0.6109(2) 0.0086(10) Uani 1 1 d U . .
O9 O 0.6132(6) 0.3428(5) 0.6463(2) 0.0082(10) Uani 1 1 d U . .
O10 O 1.3717(7) 0.7766(5) 0.8815(2) 0.0105(11) Uani 1 1 d U . .
O11 O 0.6606(7) 0.3401(5) 0.8214(2) 0.0109(11) Uani 1 1 d U . .
O12 O 1.1688(7) 0.4200(5) 0.8663(3) 0.0126(11) Uani 1 1 d U . .
O13 O 1.3641(7) 0.6883(5) 0.5226(2) 0.0091(11) Uani 1 1 d U . .
O14 O 0.8760(7) 0.2986(5) 0.8942(2) 0.0097(11) Uani 1 1 d U . .
O15 O 1.0942(7) 0.8728(5) 0.6008(2) 0.0117(12) Uani 1 1 d U . .
O16 O 1.4442(7) 0.4614(5) 0.5999(2) 0.0116(12) Uani 1 1 d U . .
O17 O 1.6363(7) 0.6969(5) 0.8807(3) 0.0120(12) Uani 1 1 d U . .
O18 O 0.3049(7) 0.3153(5) 0.6783(3) 0.0114(12) Uani 1 1 d U . .
O19 O 1.2355(8) 0.9166(5) 0.9282(2) 0.0137(12) Uani 1 1 d U . .
O20 O 0.3936(7) 0.1311(5) 0.6583(2) 0.0102(11) Uani 1 1 d U . .
O21 O 1.5605(7) 0.6887(5) 0.6177(3) 0.0167(13) Uani 1 1 d U . .
O22 O 0.5992(8) 0.8717(6) 0.7074(3) 0.0220(14) Uani 1 1 d U . .
O23 O 0.3390(8) 0.3185(6) 0.7846(3) 0.0238(15) Uani 1 1 d U . .
O24 O 0.8844(9) 1.0684(5) 0.8384(3) 0.0245(16) Uani 1 1 d U . .
O25 O 0.6234(8) 0.8745(6) 0.8160(3) 0.0227(15) Uani 1 1 d U . .
O26 O 1.5227(8) 0.4809(6) 0.8913(3) 0.0271(16) Uani 1 1 d U . .
O27 O 1.3495(9) 0.4917(7) 0.9763(4) 0.045(2) Uani 1 1 d U . .
Se10 Se 1.48736(10) 0.78738(7) 1.03432(3) 0.00942(16) Uani 1 1 d U . .
O101 O 1.4121(7) 0.7013(5) 1.0740(3) 0.0131(12) Uani 1 1 d U . .
O103 O 1.3855(8) 0.8616(5) 1.0214(3) 0.0166(14) Uani 1 1 d U . .
O102 O 1.5066(7) 0.7175(5) 0.9782(2) 0.0153(12) Uani 1 1 d U . .
O104 O 1.6651(7) 0.8656(5) 1.0616(3) 0.0175(14) Uani 1 1 d U . .
Se30 Se 1.27221(9) 0.58657(6) 0.74790(3) 0.00569(14) Uani 1 1 d U . .
O31 O 1.3593(7) 0.5800(5) 0.6947(2) 0.0106(11) Uani 1 1 d U . .
O32 O 1.2338(7) 0.7012(5) 0.7554(2) 0.0086(10) Uani 1 1 d U . .
O33 O 1.1085(7) 0.4812(5) 0.7419(2) 0.0100(10) Uani 1 1 d U . .
O34 O 1.3863(7) 0.5832(5) 0.8008(2) 0.0108(11) Uani 1 1 d U . .
Se40 Se 0.73817(9) 0.59482(6) 0.74942(3) 0.00568(14) Uani 1 1 d U . .
O41 O 0.8207(7) 0.5889(5) 0.6944(2) 0.0095(10) Uani 1 1 d U . .
O42 O 0.5817(7) 0.4877(4) 0.7441(2) 0.0083(11) Uani 1 1 d U . .
O43 O 0.8593(7) 0.5999(5) 0.8022(2) 0.0098(10) Uani 1 1 d U . .
O44 O 0.6929(7) 0.7045(5) 0.7575(3) 0.0124(12) Uani 1 1 d U . .
Se50 Se 0.86287(9) 0.17959(6) 0.72428(3) 0.00651(15) Uani 1 1 d U . .
O51 O 0.6775(6) 0.1562(5) 0.7103(2) 0.0099(11) Uani 1 1 d U . .
O52 O 0.8870(7) 1.0614(5) 0.7178(3) 0.0110(12) Uani 1 1 d U . .
O53 O 0.9629(7) 0.2511(5) 0.6828(2) 0.0096(11) Uani 1 1 d U . .
O54 O 0.9314(7) 0.2430(5) 0.7867(2) 0.0101(11) Uani 1 1 d U . .
Se60 Se 0.87322(9) 0.57107(6) 0.54632(3) 0.00578(14) Uani 1 1 d U . .
O61 O 0.8615(7) 0.6705(4) 0.5888(2) 0.0075(10) Uani 1 1 d U . .
O62 O 1.2299(7) 0.4445(5) 0.5118(2) 0.0079(11) Uani 1 1 d U . .
O63 O 0.7977(7) 0.4564(5) 0.5699(2) 0.0091(11) Uani 1 1 d U . .
O64 O 1.0553(7) 0.5963(5) 0.5384(2) 0.0106(11) Uani 1 1 d U . .
Se70 Se 0.82627(10) 0.15489(7) 0.54799(3) 0.00810(15) Uani 1 1 d U . .
O71 O 1.0151(7) 0.1859(5) 0.5538(3) 0.0136(13) Uani 1 1 d U . .
O72 O 0.7532(7) 0.1426(5) 0.4849(2) 0.0129(12) Uani 1 1 d U . .
O73 O 0.7802(7) 0.2521(5) 0.5823(2) 0.0096(11) Uani 1 1 d U . .
O74 O 0.7506(7) 0.0409(5) 0.5714(3) 0.0141(13) Uani 1 1 d U . .
Se80 Se 1.29338(9) 1.00808(6) 0.77173(3) 0.00635(15) Uani 1 1 d U . .
O81 O 1.2833(7) 0.9314(5) 0.7136(2) 0.0117(11) Uani 1 1 d U . .
O82 O 0.4315(7) 0.1259(5) 0.7776(2) 0.0114(12) Uani 1 1 d U . .
O83 O 1.3241(7) 0.9446(5) 0.8209(2) 0.0117(11) Uani 1 1 d U . .
O84 O 1.1289(7) 1.0319(5) 0.7748(2) 0.0107(11) Uani 1 1 d U . .
Se90 Se 0.99044(9) 0.62272(7) 0.95095(3) 0.00796(15) Uani 1 1 d U . .
O91 O 0.9254(7) 0.6409(5) 1.0079(2) 0.0117(12) Uani 1 1 d U . .
O92 O 0.8755(7) 0.5113(5) 0.9122(3) 0.0138(12) Uani 1 1 d U . .
O93 O 1.1656(8) 0.6188(7) 0.9622(3) 0.0260(16) Uani 1 1 d U . .
O94 O 0.9915(9) 0.7266(5) 0.9207(3) 0.0202(14) Uani 1 1 d U . .
OW1 O 0.7493(8) 0.8370(5) 0.5646(2) 0.0148(13) Uani 1 1 d . . .
OW2 O 0.4683(7) 0.9656(5) 0.6049(3) 0.0142(13) Uani 1 1 d . . .
OW3 O 0.2128(8) 0.2222(5) 0.8638(3) 0.0192(15) Uani 1 1 d . . .
OW4 O 0.3576(8) 0.2542(5) 0.5475(3) 0.0183(14) Uani 1 1 d . . .
OW5 O 1.3353(12) 1.0258(8) 1.0820(4) 0.057(3) Uani 1 1 d . . .
OW6A O 0.8446(14) 0.8534(10) 0.9697(5) 0.031(4) Uani 0.645(17) 1 d PU A 1
OW6B O 0.928(2) 0.9650(14) 0.9561(7) 0.014(5) Uani 0.355(17) 1 d PU A 2
OW7 O 0.959(2) 0.8695(14) 0.0468(7) 0.046(5) Uani 0.50 1 d P . .
OW8 O 0.0828(7) 0.0702(5) 0.6305(3) 0.0136(13) Uani 1 1 d . . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Se Se -0.0929 2.2259 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Th Th -7.2400 8.8979 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O3 Th1 O2 118.80(19) . .
O3 Th1 O12 68.3(2) . .
O2 Th1 O12 134.7(2) . .
O3 Th1 O11 141.1(2) . .
O2 Th1 O11 67.7(2) . .
O12 Th1 O11 137.5(2) . .
O3 Th1 O92 74.1(2) . .
O2 Th1 O92 132.6(2) . .
O12 Th1 O92 92.7(2) . .
O11 Th1 O92 75.8(2) . .
O3 Th1 O54 134.9(2) . .
O2 Th1 O54 72.33(19) . .
O12 Th1 O54 74.6(2) . .
O11 Th1 O54 84.0(2) . .
O92 Th1 O54 133.3(2) . .
O3 Th1 O14 118.92(19) . .
O2 Th1 O14 122.28(19) . .
O12 Th1 O14 69.4(2) . .
O11 Th1 O14 68.61(19) . .
O92 Th1 O14 66.12(19) . .
O54 Th1 O14 67.36(19) . .
O3 Th1 O43 63.93(18) . .
O2 Th1 O43 72.59(19) . .
O12 Th1 O43 132.2(2) . .
O11 Th1 O43 84.81(19) . .
O92 Th1 O43 75.03(19) . .
O54 Th1 O43 144.86(18) . .
O14 Th1 O43 136.89(18) . .
O3 Th1 O33 70.49(18) . .
O2 Th1 O33 62.29(18) . .
O12 Th1 O33 82.3(2) . .
O11 Th1 O33 129.95(19) . .
O92 Th1 O33 143.56(19) . .
O54 Th1 O33 80.22(19) . .
O14 Th1 O33 141.27(18) . .
O43 Th1 O33 81.78(18) . .
O3 Th1 Th8 32.84(13) . .
O2 Th1 Th8 137.99(14) . .
O12 Th1 Th8 35.62(14) . .
O11 Th1 Th8 153.53(14) . .
O92 Th1 Th8 79.02(15) . .
O54 Th1 Th8 107.89(14) . .
O14 Th1 Th8 93.68(13) . .
O43 Th1 Th8 96.67(13) . .
O33 Th1 Th8 76.17(12) . .
O3 Th1 Th5 140.23(13) . .
O2 Th1 Th5 32.69(14) . .
O12 Th1 Th5 148.49(15) . .
O11 Th1 Th5 35.05(14) . .
O92 Th1 Th5 106.91(15) . .
O54 Th1 Th5 74.04(13) . .
O14 Th1 Th5 95.90(13) . .
O43 Th1 Th5 77.74(13) . .
O33 Th1 Th5 94.90(12) . .
Th8 Th1 Th5 170.174(11) . .
O3 Th1 Th2 99.81(14) . .
O2 Th1 Th2 24.46(14) . .
O12 Th1 Th2 115.50(16) . .
O11 Th1 Th2 92.14(14) . .
O92 Th1 Th2 147.07(15) . .
O54 Th1 Th2 73.84(13) . .
O14 Th1 Th2 137.89(13) . .
O43 Th1 Th2 73.41(13) . .
O33 Th1 Th2 37.84(12) . .
Th8 Th1 Th2 113.690(9) . .
Th5 Th1 Th2 57.134(7) . .
O2 Th2 O1 119.05(19) . .
O2 Th2 O8 138.48(19) . .
O1 Th2 O8 67.60(19) . .
O2 Th2 O9 67.9(2) . .
O1 Th2 O9 130.48(19) . .
O8 Th2 O9 142.6(2) . .
O2 Th2 O73 114.4(2) . .
O1 Th2 O73 126.51(19) . .
O8 Th2 O73 75.0(2) . .
O9 Th2 O73 68.5(2) . .
O2 Th2 O63 135.69(19) . .
O1 Th2 O63 73.96(19) . .
O8 Th2 O63 85.73(19) . .
O9 Th2 O63 72.57(19) . .
O73 Th2 O63 66.25(19) . .
O2 Th2 O53 73.70(19) . .
O1 Th2 O53 126.79(19) . .
O8 Th2 O53 71.95(19) . .
O9 Th2 O53 102.62(19) . .
O73 Th2 O53 70.91(19) . .
O63 Th2 O53 135.50(19) . .
O2 Th2 O33 64.09(19) . .
O1 Th2 O33 71.57(18) . .
O8 Th2 O33 82.74(19) . .
O9 Th2 O33 131.49(19) . .
O73 Th2 O33 139.65(19) . .
O63 Th2 O33 145.49(19) . .
O53 Th2 O33 70.35(18) . .
O2 Th2 O41 72.20(18) . .
O1 Th2 O41 63.24(18) . .
O8 Th2 O41 130.80(19) . .
O9 Th2 O41 75.50(18) . .
O73 Th2 O41 135.84(19) . .
O63 Th2 O41 79.39(18) . .
O53 Th2 O41 143.72(18) . .
O33 Th2 O41 83.85(18) . .
O2 Th2 Th5 32.85(14) . .
O1 Th2 Th5 138.70(13) . .
O8 Th2 Th5 152.23(14) . .
O9 Th2 Th5 35.98(14) . .
O73 Th2 Th5 88.35(14) . .
O63 Th2 Th5 108.03(13) . .
O53 Th2 Th5 81.73(13) . .
O33 Th2 Th5 96.87(13) . .
O41 Th2 Th5 76.38(12) . .
O2 Th2 Th6 140.19(14) . .
O1 Th2 Th6 32.96(13) . .
O8 Th2 Th6 34.84(14) . .
O9 Th2 Th6 147.37(14) . .
O73 Th2 Th6 100.67(14) . .
O63 Th2 Th6 74.92(14) . .
O53 Th2 Th6 102.34(13) . .
O33 Th2 Th6 77.13(13) . .
O41 Th2 Th6 95.99(12) . .
Th5 Th2 Th6 170.884(10) . .
O2 Th2 Th4 101.56(14) . .
O1 Th2 Th4 23.87(13) . .
O8 Th2 Th4 91.47(14) . .
O9 Th2 Th4 110.62(13) . .
O73 Th2 Th4 138.90(14) . .
O63 Th2 Th4 74.29(14) . .
O53 Th2 Th4 141.79(13) . .
O33 Th2 Th4 73.61(13) . .
O41 Th2 Th4 39.38(12) . .
Th5 Th2 Th4 115.192(9) . .
Th6 Th2 Th4 56.755(7) . .
O4 Th3 O3 118.46(19) . .
O4 Th3 O10 137.1(2) . .
O3 Th3 O10 67.3(2) . .
O4 Th3 O5 67.1(2) . .
O3 Th3 O5 136.9(2) . .
O10 Th3 O5 140.7(2) . .
O4 Th3 O94 127.0(2) . .
O3 Th3 O94 74.9(2) . .
O10 Th3 O94 95.8(2) . .
O5 Th3 O94 70.8(2) . .
O4 Th3 O83 74.9(2) . .
O3 Th3 O83 134.3(2) . .
O10 Th3 O83 74.6(2) . .
O5 Th3 O83 88.8(2) . .
O94 Th3 O83 134.7(2) . .
O4 Th3 O19 126.46(19) . .
O3 Th3 O19 115.01(19) . .
O10 Th3 O19 68.1(2) . .
O5 Th3 O19 72.8(2) . .
O94 Th3 O19 65.4(2) . .
O83 Th3 O19 70.1(2) . .
O4 Th3 O32 65.21(18) . .
O3 Th3 O32 72.32(18) . .
O10 Th3 O32 78.78(19) . .
O5 Th3 O32 132.22(19) . .
O94 Th3 O32 146.31(19) . .
O83 Th3 O32 76.38(19) . .
O19 Th3 O32 137.6(2) . .
O4 Th3 O43 70.50(19) . .
O3 Th3 O43 62.45(18) . .
O10 Th3 O43 129.69(18) . .
O5 Th3 O43 83.29(19) . .
O94 Th3 O43 74.1(2) . .
O83 Th3 O43 144.93(18) . .
O19 Th3 O43 137.72(19) . .
O32 Th3 O43 83.93(18) . .
O4 Th3 Th8 140.00(14) . .
O3 Th3 Th8 32.66(14) . .
O10 Th3 Th8 35.09(14) . .
O5 Th3 Th8 150.38(14) . .
O94 Th3 Th8 80.26(16) . .
O83 Th3 Th8 107.95(14) . .
O19 Th3 Th8 89.71(14) . .
O32 Th3 Th8 76.55(12) . .
O43 Th3 Th8 95.01(12) . .
O4 Th3 Th7 32.36(14) . .
O3 Th3 Th7 137.74(14) . .
O10 Th3 Th7 152.65(14) . .
O5 Th3 Th7 34.84(14) . .
O94 Th3 Th7 101.50(17) . .
O83 Th3 Th7 78.14(14) . .
O19 Th3 Th7 100.24(14) . .
O32 Th3 Th7 97.38(12) . .
O43 Th3 Th7 75.95(12) . .
Th8 Th3 Th7 169.728(10) . .
O4 Th3 Th4 25.03(14) . .
O3 Th3 Th4 101.27(14) . .
O10 Th3 Th4 115.56(15) . .
O5 Th3 Th4 92.10(14) . .
O94 Th3 Th4 144.53(18) . .
O83 Th3 Th4 73.02(14) . .
O19 Th3 Th4 140.20(14) . .
O32 Th3 Th4 40.19(12) . .
O43 Th3 Th4 73.21(12) . .
Th8 Th3 Th4 115.821(9) . .
Th7 Th3 Th4 57.288(7) . .
O1 Th4 O4 118.44(19) . .
O1 Th4 O6 138.6(2) . .
O4 Th4 O6 67.1(2) . .
O1 Th4 O7 68.6(2) . .
O4 Th4 O7 134.9(2) . .
O6 Th4 O7 139.7(2) . .
O1 Th4 O81 132.2(2) . .
O4 Th4 O81 73.9(2) . .
O6 Th4 O81 89.2(2) . .
O7 Th4 O81 72.1(2) . .
O1 Th4 O15 115.97(19) . .
O4 Th4 O15 125.30(19) . .
O6 Th4 O15 69.1(2) . .
O7 Th4 O15 71.5(2) . .
O81 Th4 O15 74.4(2) . .
O1 Th4 O61 74.06(18) . .
O4 Th4 O61 126.28(19) . .
O6 Th4 O61 72.12(19) . .
O7 Th4 O61 98.76(19) . .
O81 Th4 O61 139.05(19) . .
O15 Th4 O61 65.01(19) . .
O1 Th4 O41 64.39(19) . .
O4 Th4 O41 71.87(19) . .
O6 Th4 O41 81.4(2) . .
O7 Th4 O41 132.97(18) . .
O81 Th4 O41 145.51(18) . .
O15 Th4 O41 130.73(19) . .
O61 Th4 O41 68.80(18) . .
O1 Th4 O32 71.24(18) . .
O4 Th4 O32 63.92(18) . .
O6 Th4 O32 130.96(19) . .
O7 Th4 O32 79.66(19) . .
O81 Th4 O32 75.91(19) . .
O15 Th4 O32 143.58(19) . .
O61 Th4 O32 143.23(17) . .
O41 Th4 O32 85.36(18) . .
O1 Th4 Th6 33.23(14) . .
O4 Th4 Th6 139.06(13) . .
O6 Th4 Th6 152.30(14) . .
O7 Th4 Th6 35.75(14) . .
O81 Th4 Th6 105.65(14) . .
O15 Th4 Th6 92.11(13) . .
O61 Th4 Th6 81.61(12) . .
O41 Th4 Th6 97.40(12) . .
O32 Th4 Th6 76.11(12) . .
O1 Th4 Th7 139.41(14) . .
O4 Th4 Th7 32.81(13) . .
O6 Th4 Th7 34.44(14) . .
O7 Th4 Th7 149.18(14) . .
O81 Th4 Th7 77.28(14) . .
O15 Th4 Th7 97.00(13) . .
O61 Th4 Th7 101.95(12) . .
O41 Th4 Th7 76.39(12) . .
O32 Th4 Th7 96.54(12) . .
Th6 Th4 Th7 170.881(10) . .
O1 Th4 Th3 100.38(14) . .
O4 Th4 Th3 25.00(14) . .
O6 Th4 Th3 92.06(14) . .
O7 Th4 Th3 114.25(14) . .
O81 Th4 Th3 72.18(13) . .
O15 Th4 Th3 141.64(14) . .
O61 Th4 Th3 142.14(13) . .
O41 Th4 Th3 75.05(12) . .
O32 Th4 Th3 38.92(12) . .
Th6 Th4 Th3 114.524(9) . .
Th7 Th4 Th3 57.712(7) . .
O2 Th5 O11 68.3(2) . .
O2 Th5 O9 68.43(19) . .
O11 Th5 O9 135.1(2) . .
O2 Th5 O20 124.43(19) . .
O11 Th5 O20 144.4(2) . .
O9 Th5 O20 73.57(19) . .
O2 Th5 O51 71.18(19) . .
O11 Th5 O51 92.3(2) . .
O9 Th5 O51 84.71(19) . .
O20 Th5 O51 66.27(19) . .
O2 Th5 O42 72.16(19) . .
O11 Th5 O42 79.9(2) . .
O9 Th5 O42 76.15(19) . .
O20 Th5 O42 134.31(19) . .
O51 Th5 O42 142.79(19) . .
O2 Th5 O23 131.1(2) . .
O11 Th5 O23 73.9(2) . .
O9 Th5 O23 130.7(2) . .
O20 Th5 O23 104.4(2) . .
O51 Th5 O23 141.0(2) . .
O42 Th5 O23 71.7(2) . .
O2 Th5 O82 122.51(19) . .
O11 Th5 O82 72.5(2) . .
O9 Th5 O82 144.5(2) . .
O20 Th5 O82 73.5(2) . .
O51 Th5 O82 70.2(2) . .
O42 Th5 O82 138.20(19) . .
O23 Th5 O82 70.9(2) . .
O2 Th5 O18 131.08(19) . .
O11 Th5 O18 133.3(2) . .
O9 Th5 O18 72.17(19) . .
O20 Th5 O18 67.41(19) . .
O51 Th5 O18 132.36(19) . .
O42 Th5 O18 71.21(19) . .
O23 Th5 O18 62.7(2) . .
O82 Th5 O18 106.41(19) . .
O2 Th5 Th2 32.77(14) . .
O11 Th5 Th2 101.07(15) . .
O9 Th5 Th2 36.61(13) . .
O20 Th5 Th2 97.35(14) . .
O51 Th5 Th2 69.10(13) . .
O42 Th5 Th2 76.72(13) . .
O23 Th5 Th2 148.39(18) . .
O82 Th5 Th2 138.47(14) . .
O18 Th5 Th2 106.85(13) . .
O2 Th5 Th1 32.73(14) . .
O11 Th5 Th1 35.64(15) . .
O9 Th5 Th1 100.77(14) . .
O20 Th5 Th1 144.34(14) . .
O51 Th5 Th1 78.24(13) . .
O42 Th5 Th1 74.49(14) . .
O23 Th5 Th1 105.29(17) . .
O82 Th5 Th1 98.26(14) . .
O18 Th5 Th1 145.69(13) . .
Th2 Th5 Th1 65.484(9) . .
O1 Th6 O8 68.35(19) . .
O1 Th6 O7 68.4(2) . .
O8 Th6 O7 136.1(2) . .
O1 Th6 O64 70.95(19) . .
O8 Th6 O64 92.6(2) . .
O7 Th6 O64 80.3(2) . .
O1 Th6 O31 72.70(19) . .
O8 Th6 O31 79.4(2) . .
O7 Th6 O31 81.1(2) . .
O64 Th6 O31 143.15(19) . .
O1 Th6 O62 124.6(2) . .
O8 Th6 O62 71.79(19) . .
O7 Th6 O62 143.33(19) . .
O64 Th6 O62 74.21(19) . .
O31 Th6 O62 134.12(18) . .
O1 Th6 O16 132.02(19) . .
O8 Th6 O16 73.7(2) . .
O7 Th6 O16 135.1(2) . .
O64 Th6 O16 139.9(2) . .
O31 Th6 O16 72.37(19) . .
O62 Th6 O16 65.77(19) . .
O1 Th6 O21 129.9(2) . .
O8 Th6 O21 135.0(2) . .
O7 Th6 O21 72.4(2) . .
O64 Th6 O21 130.8(2) . .
O31 Th6 O21 71.5(2) . .
O62 Th6 O21 105.4(2) . .
O16 Th6 O21 65.2(2) . .
O1 Th6 O13 126.85(19) . .
O8 Th6 O13 141.45(19) . .
O7 Th6 O13 74.37(19) . .
O64 Th6 O13 66.41(19) . .
O31 Th6 O13 136.6(2) . .
O62 Th6 O13 71.46(18) . .
O16 Th6 O13 101.13(18) . .
O21 Th6 O13 67.2(2) . .
O1 Th6 Th4 32.56(13) . .
O8 Th6 Th4 100.91(14) . .
O7 Th6 Th4 36.27(15) . .
O64 Th6 Th4 68.43(14) . .
O31 Th6 Th4 77.79(13) . .
O62 Th6 Th4 141.60(13) . .
O16 Th6 Th4 150.16(13) . .
O21 Th6 Th4 105.44(14) . .
O13 Th6 Th4 100.53(13) . .
O1 Th6 Th2 33.14(14) . .
O8 Th6 Th2 35.41(14) . .
O7 Th6 Th2 101.55(15) . .
O64 Th6 Th2 77.21(14) . .
O31 Th6 Th2 75.76(14) . .
O62 Th6 Th2 98.07(14) . .
O16 Th6 Th2 105.98(14) . .
O21 Th6 Th2 147.26(15) . .
O13 Th6 Th2 143.59(13) . .
Th4 Th6 Th2 65.642(9) . .
O4 Th7 O6 68.0(2) . .
O4 Th7 O5 68.1(2) . .
O6 Th7 O5 136.0(2) . .
O4 Th7 O84 73.32(19) . .
O6 Th7 O84 86.8(2) . .
O5 Th7 O84 83.6(2) . .
O4 Th7 O44 72.5(2) . .
O6 Th7 O44 81.8(2) . .
O5 Th7 O44 82.5(2) . .
O84 Th7 O44 145.80(19) . .
O4 Th7 O52 123.9(2) . .
O6 Th7 O52 72.6(2) . .
O5 Th7 O52 138.2(2) . .
O84 Th7 O52 66.02(19) . .
O44 Th7 O52 138.2(2) . .
O4 Th7 O25 129.5(2) . .
O6 Th7 O25 131.5(2) . .
O5 Th7 O25 77.4(2) . .
O84 Th7 O25 138.6(2) . .
O44 Th7 O25 67.3(2) . .
O52 Th7 O25 106.5(2) . .
O4 Th7 O24 129.6(2) . .
O6 Th7 O24 144.4(2) . .
O5 Th7 O24 71.8(2) . .
O84 Th7 O24 73.2(2) . .
O44 Th7 O24 130.4(2) . .
O52 Th7 O24 72.4(2) . .
O25 Th7 O24 66.1(2) . .
O4 Th7 O22 129.1(2) . .
O6 Th7 O22 72.2(2) . .
O5 Th7 O22 138.6(2) . .
O84 Th7 O22 134.6(2) . .
O44 Th7 O22 71.6(2) . .
O52 Th7 O22 69.4(2) . .
O25 Th7 O22 63.2(2) . .
O24 Th7 O22 101.1(2) . .
O4 Th7 Th4 32.78(14) . .
O6 Th7 Th4 35.44(15) . .
O5 Th7 Th4 100.86(14) . .
O84 Th7 Th4 75.27(13) . .
O44 Th7 Th4 76.90(14) . .
O52 Th7 Th4 98.36(14) . .
O25 Th7 Th4 144.13(17) . .
O24 Th7 Th4 148.19(18) . .
O22 Th7 Th4 103.81(15) . .
O4 Th7 Th3 32.30(14) . .
O6 Th7 Th3 100.34(15) . .
O5 Th7 Th3 35.89(14) . .
O84 Th7 Th3 73.88(13) . .
O44 Th7 Th3 76.58(14) . .
O52 Th7 Th3 139.48(14) . .
O25 Th7 Th3 107.21(16) . .
O24 Th7 Th3 101.88(17) . .
O22 Th7 Th3 147.99(17) . .
Th4 Th7 Th3 65.000(9) . .
O3 Th8 O10 67.7(2) . .
O3 Th8 O12 68.4(2) . .
O10 Th8 O12 135.4(2) . .
O3 Th8 O102 130.2(2) . .
O10 Th8 O102 76.5(2) . .
O12 Th8 O102 142.2(2) . .
O3 Th8 O34 73.19(19) . .
O10 Th8 O34 79.3(2) . .
O12 Th8 O34 80.7(2) . .
O102 Th8 O34 132.9(2) . .
O3 Th8 O93 70.8(2) . .
O10 Th8 O93 86.8(2) . .
O12 Th8 O93 86.5(2) . .
O102 Th8 O93 73.8(2) . .
O34 Th8 O93 144.0(2) . .
O3 Th8 O27 123.5(2) . .
O10 Th8 O27 141.2(3) . .
O12 Th8 O27 73.4(3) . .
O102 Th8 O27 69.3(3) . .
O34 Th8 O27 138.2(3) . .
O93 Th8 O27 66.8(3) . .
O3 Th8 O26 136.6(2) . .
O10 Th8 O26 135.7(2) . .
O12 Th8 O26 76.2(2) . .
O102 Th8 O26 93.2(2) . .
O34 Th8 O26 77.0(2) . .
O93 Th8 O26 132.1(2) . .
O27 Th8 O26 65.4(3) . .
O3 Th8 O17 126.93(19) . .
O10 Th8 O17 72.8(2) . .
O12 Th8 O17 131.5(2) . .
O102 Th8 O17 68.8(2) . .
O34 Th8 O17 65.7(2) . .
O93 Th8 O17 140.5(2) . .
O27 Th8 O17 109.5(2) . .
O26 Th8 O17 63.4(2) . .
O3 Th8 Th1 33.04(14) . .
O10 Th8 Th1 100.73(14) . .
O12 Th8 Th1 35.56(14) . .
O102 Th8 Th1 147.13(15) . .
O34 Th8 Th1 76.88(14) . .
O93 Th8 Th1 73.31(16) . .
O27 Th8 Th1 98.34(17) . .
O26 Th8 Th1 109.54(17) . .
O17 Th8 Th1 142.55(14) . .
O3 Th8 Th3 32.88(14) . .
O10 Th8 Th3 35.30(14) . .
O12 Th8 Th3 101.26(14) . .
O102 Th8 Th3 102.92(16) . .
O34 Th8 Th3 77.41(13) . .
O93 Th8 Th3 72.31(17) . .
O27 Th8 Th3 139.0(2) . .
O26 Th8 Th3 154.39(18) . .
O17 Th8 Th3 103.98(13) . .
Th1 Th8 Th3 65.860(9) . .
Th4 O1 Th6 114.2(2) . .
Th4 O1 Th2 131.7(2) . .
Th6 O1 Th2 113.9(2) . .
Th2 O2 Th5 114.4(2) . .
Th2 O2 Th1 131.0(2) . .
Th5 O2 Th1 114.6(2) . .
Th8 O3 Th1 114.1(2) . .
Th8 O3 Th3 114.5(2) . .
Th1 O3 Th3 131.2(2) . .
Th3 O4 Th4 130.0(2) . .
Th3 O4 Th7 115.3(2) . .
Th4 O4 Th7 114.4(2) . .
Th7 O5 Th3 109.3(2) . .
Th7 O6 Th4 110.1(2) . .
Th6 O7 Th4 108.0(2) . .
Th6 O8 Th2 109.8(2) . .
Th5 O9 Th2 107.4(2) . .
Th8 O10 Th3 109.6(2) . .
Th5 O11 Th1 109.3(2) . .
Th1 O12 Th8 108.8(2) . .
O103 Se10 O101 113.0(3) . .
O103 Se10 O102 110.7(3) . .
O101 Se10 O102 108.0(3) . .
O103 Se10 O104 110.1(3) . .
O101 Se10 O104 109.3(3) . .
O102 Se10 O104 105.5(3) . .
Se10 O102 Th8 139.6(3) . .
O31 Se30 O34 108.7(3) . .
O31 Se30 O33 110.9(3) . .
O34 Se30 O33 108.0(3) . .
O31 Se30 O32 109.1(3) . .
O34 Se30 O32 110.8(3) . .
O33 Se30 O32 109.3(3) . .
Se30 O31 Th6 129.6(3) . .
Se30 O32 Th3 123.9(3) . .
Se30 O32 Th4 122.0(3) . .
Th3 O32 Th4 100.89(18) . .
Se30 O33 Th2 124.6(3) . .
Se30 O33 Th1 124.0(3) . .
Th2 O33 Th1 102.60(19) . .
Se30 O34 Th8 129.5(3) . .
O42 Se40 O44 109.4(3) . .
O42 Se40 O43 109.8(3) . .
O44 Se40 O43 108.7(3) . .
O42 Se40 O41 109.6(3) . .
O44 Se40 O41 109.7(3) . .
O43 Se40 O41 109.7(3) . .
Se40 O41 Th4 123.6(3) . .
Se40 O41 Th2 122.2(3) . .
Th4 O41 Th2 100.67(18) . .
Se40 O42 Th5 131.3(3) . .
Se40 O43 Th1 124.1(3) . .
Se40 O43 Th3 124.4(3) . .
Th1 O43 Th3 102.39(19) . .
Se40 O44 Th7 130.1(3) . .
O51 Se50 O53 111.8(3) . .
O51 Se50 O52 107.8(3) . 1_545
O53 Se50 O52 108.2(3) . 1_545
O51 Se50 O54 111.7(3) . .
O53 Se50 O54 109.1(3) . .
O52 Se50 O54 108.2(3) 1_545 .
Se50 O51 Th5 126.9(3) . .
Se50 O52 Th7 141.5(3) 1_565 .
Se50 O53 Th2 119.2(3) . .
Se50 O54 Th1 125.2(3) . .
O62 Se60 O61 111.6(3) 2_766 .
O62 Se60 O64 109.8(3) 2_766 .
O61 Se60 O64 109.0(3) . .
O62 Se60 O63 105.9(3) 2_766 .
O61 Se60 O63 108.4(3) . .
O64 Se60 O63 112.2(3) . .
Se60 O61 Th4 119.2(3) . .
Se60 O62 Th6 130.8(3) 2_766 .
Se60 O63 Th2 126.2(3) . .
Se60 O64 Th6 129.3(3) . .
O72 Se70 O71 110.8(3) . .
O72 Se70 O74 110.9(3) . .
O71 Se70 O74 108.4(3) . .
O72 Se70 O73 106.2(3) . .
O71 Se70 O73 111.3(3) . .
O74 Se70 O73 109.3(3) . .
Se70 O73 Th2 140.4(3) . .
O82 Se80 O83 110.2(3) 1_665 .
O82 Se80 O81 110.8(3) 1_665 .
O83 Se80 O81 108.8(3) . .
O82 Se80 O84 106.9(3) 1_665 .
O83 Se80 O84 110.3(3) . .
O81 Se80 O84 109.8(3) . .
Se80 O81 Th4 126.0(3) . .
Se80 O82 Th5 143.4(3) 1_445 .
Se80 O83 Th3 124.2(3) . .
Se80 O84 Th7 129.3(3) . .
O91 Se90 O92 111.1(3) . .
O91 Se90 O93 110.0(3) . .
O92 Se90 O93 110.2(4) . .
O91 Se90 O94 106.5(3) . .
O92 Se90 O94 108.0(3) . .
O93 Se90 O94 111.0(4) . .
Se90 O92 Th1 124.5(3) . .
Se90 O93 Th8 130.5(3) . .
Se90 O94 Th3 124.2(3) . .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Th1 O3 2.307(6) .
Th1 O2 2.310(6) .
Th1 O12 2.373(6) .
Th1 O11 2.399(6) .
Th1 O92 2.509(6) .
Th1 O54 2.531(6) .
Th1 O14 2.597(6) .
Th1 O43 2.654(6) .
Th1 O33 2.740(6) .
Th1 Th8 3.8620(5) .
Th1 Th5 3.8861(5) .
Th1 Th2 4.1978(5) .
Th2 O2 2.303(5) .
Th2 O1 2.324(6) .
Th2 O8 2.393(6) .
Th2 O9 2.422(6) .
Th2 O73 2.469(6) .
Th2 O63 2.477(6) .
Th2 O53 2.557(6) .
Th2 O33 2.639(6) .
Th2 O41 2.740(6) .
Th2 Th5 3.8753(4) .
Th2 Th6 3.8867(4) .
Th2 Th4 4.1934(5) .
Th3 O4 2.301(6) .
Th3 O3 2.308(5) .
Th3 O10 2.375(6) .
Th3 O5 2.417(6) .
Th3 O94 2.466(6) .
Th3 O83 2.521(6) .
Th3 O19 2.558(6) .
Th3 O32 2.669(6) .
Th3 O43 2.740(6) .
Th3 Th8 3.8707(4) .
Th3 Th7 3.8917(4) .
Th3 Th4 4.1722(5) .
Th4 O1 2.272(5) .
Th4 O4 2.303(6) .
Th4 O6 2.392(6) .
Th4 O7 2.395(6) .
Th4 O81 2.514(6) .
Th4 O15 2.544(6) .
Th4 O61 2.592(6) .
Th4 O41 2.707(6) .
Th4 O32 2.742(6) .
Th4 Th6 3.8498(4) .
Th4 Th7 3.8734(4) .
Th5 O2 2.308(6) .
Th5 O11 2.365(6) .
Th5 O9 2.386(6) .
Th5 O20 2.475(6) .
Th5 O51 2.496(6) .
Th5 O42 2.499(6) .
Th5 O23 2.517(7) .
Th5 O82 2.539(6) .
Th5 O18 2.595(6) .
Th6 O1 2.313(6) .
Th6 O8 2.359(6) .
Th6 O7 2.365(6) .
Th6 O64 2.468(6) .
Th6 O31 2.483(6) .
Th6 O62 2.525(5) .
Th6 O16 2.579(6) .
Th6 O21 2.583(6) .
Th6 O13 2.601(6) .
Th7 O4 2.305(5) .
Th7 O6 2.333(6) .
Th7 O5 2.355(6) .
Th7 O84 2.449(6) .
Th7 O44 2.510(6) .
Th7 O52 2.527(6) .
Th7 O25 2.559(6) .
Th7 O24 2.591(6) .
Th7 O22 2.618(7) .
Th8 O3 2.295(6) .
Th8 O10 2.362(6) .
Th8 O12 2.376(6) .
Th8 O102 2.397(6) .
Th8 O34 2.488(6) .
Th8 O93 2.490(7) .
Th8 O27 2.575(7) .
Th8 O26 2.592(7) .
Th8 O17 2.622(6) .
Se10 O103 1.611(6) .
Se10 O101 1.626(6) .
Se10 O102 1.642(6) .
Se10 O104 1.643(6) .
Se30 O31 1.628(6) .
Se30 O34 1.637(6) .
Se30 O33 1.649(6) .
Se30 O32 1.658(6) .
Se40 O42 1.623(6) .
Se40 O44 1.629(6) .
Se40 O43 1.638(6) .
Se40 O41 1.642(6) .
Se50 O51 1.629(6) .
Se50 O53 1.629(6) .
Se50 O52 1.638(6) 1_545
Se50 O54 1.642(6) .
O52 Se50 1.638(6) 1_565
Se60 O62 1.622(6) 2_766
Se60 O61 1.622(5) .
Se60 O64 1.633(6) .
Se60 O63 1.646(6) .
O62 Se60 1.622(6) 2_766
Se70 O72 1.633(6) .
Se70 O71 1.637(6) .
Se70 O74 1.637(6) .
Se70 O73 1.649(6) .
Se80 O82 1.621(6) 1_665
Se80 O83 1.636(6) .
Se80 O81 1.644(6) .
Se80 O84 1.656(6) .
O82 Se80 1.621(6) 1_445
Se90 O91 1.622(6) .
Se90 O92 1.622(6) .
Se90 O93 1.635(7) .
Se90 O94 1.646(6) .
